  Sn$_{0.97-y}$Co$_{0.03}$Ni$_{y}$O$_{2}$ (0 $\leq y \leq$ 0.04) nanocrystals,
with average crystallite size in the range of 7.3 nm ($y$=0.00) to 5.6 nm
($y$=0.04), have been synthesized using pH-controlled chemical co-precipitation
technique. The non-stoichiometric Sn related defects and the O related
stoichiometric Frenkel defects arising in the nanocrystals because of co-doping
have been identified and their effect on the structural and optical properties
of the nanocrystals have been extensively studied. It has been observed, using
XPS that on increasing the Ni co-doping concentration ($y$), the
non-stoichiometric Sn defect Sn$_{\text{Sn}}^{"}$ increases in compensation of
existing defect Sn$_{i}^{....}$ for $y$ = 0.00 nanocrystals. High resolution
transmission electron microscopy (HR-TEM) also confirms the existence of
Sn$_{\text{Sn}}^{"}$. Regarding the Frenkel defect, XPS results indicate that
the concentration of $V_{\text{O}}$ and O$_{i}$, manifested in the form of
dangling bond related surface defect states,increases with increase in $y$.
Temperature dependent magnetisation measurement of the nanocrystals confirm the
charge state of $V_{\text{O}}$. The point defects have been found to affect the
structural properties in a way that distortion in octahedral geometry of
complete Sn-O octahderon effectively reduces whereas distortion in the trigonal
planar coordination geometry of O increases. The investigation of Urbach edge
indicates an enhancement in the disorder in the nanocrystals on co-doping. The
optical band gap of the nanocrystals has been found to be red shifted upto
$y$=0.02 and then a gradual blue shift has been observed. A direct effect of
the O related defect has been observed on the blue luminescence of the
nanocrystals such that the spectral contribution of blue luminescence in the
total emission intensity increases by 72% for $y$=0.04 as compared to $y$=0.00.
